arxiv: v2 [condmat.suprcon] 30 Sep 2018


 Derick Kelley
 11 days ago
 Views:
Transcription
1 Firstprinciples prediction of phononmediated superconductivity in XBC (X= Mg, Ca, Sr, Ba) Enamul Haque and M. Anwar Hossain Department of Physics, Mawlana Bhashani Science and Technology University Santosh, Tangail1902, Bangladesh arxiv: v2 [condmat.suprcon] 30 Sep 2018 Catherine Stampfl School of Physics, The University of Sydney, Sydney, New South Wales, 2006, Australia. (Dated: October 2, 2018) From firstprinciples calculations, we predict four new intercalated hexagonal XBC (X=Mg, Ca, Sr, Ba) compounds to be dynamically stable and phononmediated superconductors. These compounds form a LiBC like structure but are metallic. The calculated superconducting critical temperature, T c, of MgBC is 51 K. The strong attractive interaction between σbonding electrons and the B 1g phonon mode gives rise to a larger electronphonon coupling constant (1.135) and hence high T c; notably, higher than that of MgB 2. The other compounds have a low superconducting critical temperature (417 K) due to the interaction between σbonding electrons and low energy phonons (E 2u modes). Due to their energetic and dynamic stability, we envisage that these compounds can be synthesized experimentally. PACS numbers: dk, Kc, kd, Pq, b Hexagonal layered MgB 2 is a wellknown phononmediated superconductor with a T c = 39 K [1]. In MgB 2, the σband crosses the Fermi level and hybridization with other conduction electrons is weak. The high T c state of this material develops from the strong attractive interaction between the electrons of the σband and the E 2g mode of vibrations. Likely MgB 2, materials intercalated with alkali (earth) metals show superconductivity with T c much smaller than that of MgB 2 [2 13]. Many studies have proposed possible ways to improve the transition temperature through carbon (or others) doping [14? 16]. However, the T c has not been found to improve significantly [14 19]. The T c decreases on carbon substitution of B in MgB 2 due to the introduction simultaneous disorder by carbon [16, 18, 20, 21]. Thus, it may be an alternative to examine the superconducting properties by synthesizing pure MgBC compounds. From the firstprinciples investigations of LiBC with holedoping, it was found to exhibit superconductivity below 100 K [22]. Unfortunately, experimentalists have not identified superconductivity in it due to induced structural distortions [23 27]. This is a similar effect to that of carbon doping in MgB 2. Recently, LiB 1+x C 1 x materials have been predicted to be superconductors, like MgB 2 [28]. Also on the basis of firstprinciples calculations, Gao et al. reported Li 3 B 4 C 2 (also Li 2 B 3 C) to be MgB 2 like superconductor with T c 53 K [27]. Since then, another phase, Li 4 B 5 C 3, has been reported from ab initio studies to be a superconductor with a transition temperature of 16.8 K [29]. From the firstprinciples study of NaB 1+x C 1 x, Miao et al. predicted that it would be more promising superconductor than LiB 1 x C x [30]. Like LiBC, Ravindran et al. predicted that holedoped MgB 2 C 2 is a potential superconducting material [31]. Since highquality single crystals of LiBC have already been synthesized [16,17], it may be possible to synthesize XBC (X=Mg, Ca, Sr, Ba). In the present paper, we report, using the firstprinciples calculations, four new superconducting stoichiometric compounds (XBC (X=Mg, Ca, Sr, Ba)) that are dynamically stable and may be synthesized from constituent elemental solids. We find that strong electronphonon interactions exist in all these materials. The MgBC structure has a predicted T c ( 51 K) higher than that of MgB 2 ; while SrBC and BaBC have a superconducting state below 17 K (The CaBC structure has very small T c (4 K)). FIG. 1. The ground state crystal structure of XBC (X=Mg, Ca, Sr, Ba). The X, B, and C atoms are indicated by cyan, yellow, and red spheres, respectively.
2 2 FIG. 2. Electronic band structure of the four compounds: (a) MgBC, (b) CaBC, (c) SrBC, and (d) BaBC. The Fermi level is the zero of energy. The blue and red curves with symbols represent the energy bands that cross the Fermi level and form the Fermi surface. We have selected highsymmetry kpoints in the Brillouin zone and the values of them in fractional coordinates are Γ(0, 0, 0), M (1/2,0,0), K (1/3,1/3,0), A (0,0,1/2), L (1/2,0,1/2), and H (1/3,1/3,1/2). All calculations were performed using the plane wave pseudopotential approach and the generalized gradient approximation of PerdewBurkeErnzerhof (PBEGGA) [32, 33] for the exchange correlation functional, as implemented in Quantum Espresso [34]. We use the ultrasoft pseudopotentials of Vanderbilt [35] and perform full structural relaxation. After optimizing the kpoint mesh and cutoff energy, we selected a kpoint mesh for selfconsistent field calculations, a 50 Ry cutoff energy for the wave functions, and a 400 Ry energy cutoff for the charge density. For the phonon calculations, we use a 662 grid of uniform qpoints and the same kpoint mesh as above [36]. We used a finer kpoint mesh for the calculation of the electronphonon (eph) linewidth and eph coupling constants employing the optimized tetrahedron method in eph calculation [37]. We performed the phonon calculations using density functional perturbation theory (DFPT) of linear response [38]. For the electronphonon coupling constant (EPC) calculations, we used the MigdalEliashberg formulism [39]. In this formulism, the Eliashberg spectral function is defined as [40, 41] α 2 F (ω) = 1 2πN(E F ) qv δ(ω ω qv ) γ qv hω qv (1) where N(E F ) is the density of states at the Fermi level
3 3 TABLE I. Calculated fully relaxed lattice parameters of MgB 2 and XBC of (X=Mg, Ca, Sr, Ba). Compounds a(å) c/a MgB MgBC CaBC SrBC BaBC FIG. 3. Calculated total density of states (DOS) of XBC (X=Mg, Ca, Sr, Ba) within the energy range from 4 to 4. The Fermi level is the zero of energy and indicated by the vertical dashed line. and γ qv is the electronphonon linewidth for wave vectors q and v. The EPC is determined by [40, 41] α 2 F (ω) = 2 dω. (2) ω Using the calculated EPC, the superconducting transition temperature is evaluated by the AllenDynes equation [40, 41] T c = ω ln 1.2 exp [ ] ( 1.04(1 + λ)) (λ(1 0.62µ ) µ ) (3) where µ stands for the Coulomb pseudopotential constant and its value ranges between 0.1 and 0.15 [42, 43]. ω ln stands for the logarithmic average frequency and is defined as [40, 41] [ ] 2 dω ω ln = exp λ ω α2 F (ω)ln(ω). (4) The crystal structure of XBC (X=Mg, Ca, Sr, Ba) is similar to that of MgB 2. X atoms have no bonds with either B or C. Boron and carbon are bonded together in a primitive fashion. Unlike MgB 2, the unit cell contains six equivalent atoms, two of each species. Figure 1 shows the hexagonal crystal structure of XBC (X=Mg, Ca, Sr, Ba). Our theoretical value of the lattice parameters of MgB 2 is in a good agreement with the experimental value (a = 3.086Å and c/a = 1.42) [1], as listed in table 1. The fully relaxed lattice constant along the aaxis is close to the value of MgB 2 while that along the caxis of all compounds become around twice that of MgB 2 (see Table 1). We have found that all the studied compounds are energetically stable [44]. The electronic band structures of the four compounds are shown in figure 2. All the compounds possess metallic character. We see that two energy bands cross the Fermi level and form the Fermi surface for all materials. The symbols, σ and π, indicate the type of bonding electrons belonging to the energy bands crossing the Fermi level. These bands are highly dispersive along all directions except LH. These bands are slightly flat along AL above E F and LH below E F. The bands crossing the Fermi level are doubly degenerate along the ΓA direction. If we compare the band structure of MgBC and CaBC, we see that the Fermi level in CaBC is shifted to higher energy than that of MgBC. Therefore, this may lead to a reduction of T c or eliminate the superconducting state of CaBC. However, the shift in energy of SrBC and BaBC is small as compared to CaBC. Figure 3 shows the calculated total density of states of XBC (X=Mg, Ca, Sr, Ba). The density of states at the Fermi level has increased significantly in all the studied compounds compared to MgB 2. In the case of CaBC, the DOS at the Fermi level is similar to MgBC and notably lower than both of SrBC and BaBC. As mentioned above, the DOS of MgBC at the Fermi level is much increased in comparison with that of MgB 2 for the electron injected by carbon [45]. Since the σband crosses the Fermi level, σbonding electrons can strongly attract certain modes of vibration, like the E 2g mode of MgB 2. Therefore, all compounds should be superconductors at a certain temperature. We will now investigate the electronphonon coupling within MigdalEliashberg formulism. The dynamical stability of a crystal is an important criterion in order to be able to synthesize it. Many researchers have reported the failure of synthesis of potentially promising materials due to dynamical instability [46]. The phonons determine the dynamical stability of a crystal; if any imaginary frequencies appears in the phonon band structure, the crystal structure is dynamically unstable. Recently, Kato et al.
4 4 FIG. 4. Phonon dispersion relations, total, and atom projected phonon density of states of MgBC (top panel) and CaBC (bottom panel). The blue shaded area indicates the modes of the region where electrons are strongly coupled. FIG. 5. Phonon band structures, total, and atom projected phonon density of states of SrBC (top panel) and BaBC (bottom panel). The blue shaded area indicates the modes of the region (E 2u) where electrons are strongly coupled. reported the possibility of MgB 2 like superconductivity in MgBY (Y =C, Be, Li) from electronic band structure analysis without considering the dynamical stability of these compounds [47]. They also predicted that MgBC might not be a twoband superconductor because the σband is completely filled. We note that the lattice constant of dynamically stable MgBC along the caxis is twice as large as that of considered the one in their study [47], i.e., it has different atomic structure. The Fermi level in MgBC is raised to higher energy, even around the sigma antibonding states, compared to that of MgB 2. In this respect, MgBC is different in electronic structure to that of MgB 2. Figure 4 shows the phonon dispersion relation and phonon density of states (DOS) of MgBC (upper panel) and CaBC (lower panel). We see that no imaginary frequency appears in the phonon band structure for both compounds. Therefore, hexagonal MgBC and CaBC are dynamically stable [48]. Low energy phonons mainly arise from Mg and Ca in MgBC, and CaBC respectively. Higher energy phonons arise from B and C in both compounds. In MgBC, the optical Γcenter modes are shifted to higher frequencies as compared to MgB 2. In contrast to MgB 2 (where the inplane boron mode is E 2g ), the BC inplane phonon at the
5 5 Γpoint is the B 1g mode where electrons are strongly coupled, as indicated by the shaded area in figure 4. The shaded area corresponds to the highest peak region in the Eliashberg spectral function. The corresponding frequency of the B 1g mode at the Γpoint is 495 cm 1, which is much smaller than that of the value of 692 cm 1 for MgB 2 [49]. For CaBC, low energy phonons of the E 2u mode region arise from Ca atom and in this region, electrons are strongly coupled (maximum peak region in the Eliashberg spectral function). Higher energy phonons arising from B and C have very small contributions to electronphonon interactions. Since the density of states (DOS) at the Fermi level of CaBC (see figure 3) is reduced as compared to MgBC, and the phonon frequency too (blue shaded region), σband electrons are not so strongly coupled with E 2u modes of the phonons as like in MgB 2. Therefore, CaBC cannot be a MgB 2 like superconductor. The phonon energy of the blue shaded area at Γ point is more reduced in SrBC and BaBC compared to CaBC, as shown in figure 5. Like CaBC, SrBC, and BaBC have E 2u modes region where electrons are strongly coupled. However, unlike CaBC, the density of states of SrBC and BaBC at the Fermi level are notably higher. Therefore, electrons should be more strongly coupled than those in CaBC. For hexagonal SrBC and BaBC, we do not obtain any imaginary frequencies. Therefore, both structures are energetically [44] and dynamically stable [48]. The phonon density of states of MgBC exhibits three distinct peaks; in contrast MgB 2 has only one peak [18]. The first peak arises from the Mg of E 1u mode and the second and third peaks arise from B and C. The second peak shows that Bhas a dominant contribution. The Eliashberg spectral function of MgBC also shows three peaks, in comparison with just one peak of MgB 2. The main peak around 694 cm 1 arises from the predominant interaction between σband electrons and the B 1g phonon mode. These three peaks in the Eliashberg spectral function are shifted to lower energy phonons (E 2u ) in the case of the other remaining three compounds. For CaBC, the highest peak height is almost half of the highest peak height for MgBC, SrBC, and BaBC. From the Eliashberg spectral function, we can calculate the electronphonon coupling constant, logarithmic average phonon frequency and hence the superconducting transition temperature using the AllenDynes equation [41]. Our calculated superconducting parameters of the four compounds are listed in Table 2. In the table, we have used the value of the Coulomb pseudopotential to be 0.1. For MgB 2, our calculated electronphonon coupling constant (λ) is 0.844, in a good agreement with the available results [27, 49] but slightly smaller than that of the value reported in Ref. [50]. This value is slightly larger than that of the obtained value by using Wannier in FIG. 6. Calculated Eliashberg spectral function α 2 F (ω) of MgB 2 and MgBC (upper panel), and of CaBC, SrBC, BaBC (middle panel). The lower panel shows calculated superconducting transition temperature as a function of µ. TABLE II. Calculated superconducting parameters of fully relaxed structures XBC of (X=Mg, Ca, Sr, Ba). We have used the value of to be 0.1 in Eqn. (3). Compounds ω ln (K) λ T c(k) MgBC CaBC SrBC BaBC terpolation method [51 53]. We find that the logarithmic average phonon frequency (ω ln ) is 708 K, in a good agreement with available data [27, 49, 54 58]. We obtain T c = 37K by using µ = 0.1, slightly smaller than that of the experimental value (39 K). We see that the maximum superconducting transition temperature is obtained for MgBC and minimum for CaBC. The electronphonon coupling constant (1.135) of MgBC is a 26% larger than
6 6 that obtained for MgB 2 ( ) [27, 49, 50]. Thus, if we use the value of µ to be 0, we obtain T c =72 K for MgBC. Even if we use the value of 0.15 for µ, we still obtain a superconducting transition temperature above 40 K. Therefore, MgBC is a phononmediated superconductor with larger electronphonon coupling constant and higher transition temperature than MgB 2. The larger electronphonon coupling constant of MgBC arises from three peaks in the phonon density of states, mainly due to the strong coupling of σband electrons with the B 1g phonon mode. The others three compounds have a lower transition temperature compared to MgB 2. In summary, we have predicted four new superconductors using the firstprinciples calculations. Hexagonal XBC (X=Mg, Ca, Sr, Ba) compounds are found to be phononmediated superconductors. Among these compounds, the calculated T c of MgBC is 51 K. The strong coupling between σbonding electrons and the B 1g phonon mode gives rise to a larger electronphonon coupling and hence high T c. Thus, MgBC is a superconductor with T c higher than that of MgB 2. The other compounds have a low superconducting transition temperature due to the interaction between σbonding electrons and low energy phonons (E 2u modes). We must thank W.E Pickett for giving some helpful suggestions and critical reading of the manuscript. [1] J. Nagamatsu, N. Nakagawa, T. Muranaka, Y. Zenitani, and J. Akimitsu, nature 410, 63 (2001). [2] N. Hannay, T. Geballe, B. Matthias, K. Andres, P. Schmidt, and D. MacNair, Physical Review Letters 14, 225 (1965). [3] I. Belash, A. Bronnikov, O. Zharikov, and A. Pal nichenko, Solid State Communications 69, 921 (1989). [4] N. Emery, C. Hérold, M. dastuto, V. Garcia, C. Bellin, J. Marêché, P. Lagrange, and G. Loupias, Physical Review Letters 95, (2005). [5] M. Calandra and F. Mauri, Physical Review Letters 95, (2005). [6] G. Csányi, P. Littlewood, A. H. Nevidomskyy, C. J. Pickard, and B. Simons, Nature Physics 1, 42 (2005). [7] G. Profeta, M. Calandra, and F. Mauri, Nature Physics 8, 131 (2012). [8] A. Sanna, G. Profeta, A. Floris, A. Marini, E. Gross, and S. Massidda, Physical Review B 75, (2007). [9] A. Gauzzi, S. Takashima, N. Takeshita, C. Terakura, H. Takagi, N. Emery, C. Hérold, P. Lagrange, and G. Loupias, Physical Review Letters 98, (2007). [10] A. P. Tiwari, S. Shin, E. Hwang, S.G. Jung, T. Park, and H. Lee, Journal of Physics: Condensed Matter 29, (2017). [11] S. Nishiyama, H. Fujita, M. Hoshi, X. Miao, T. Terao, X. Yang, T. Miyazaki, H. Goto, T. Kagayama, K. Shimizu, et al., Scientific Reports 7, 7436 (2017). [12] J.H. Liao, Y.C. Zhao, Y.J. Zhao, H. Xu, and X.B. Yang, Physical Chemistry Chemical Physics 19, (2017). [13] S. A. Tawfik, C. Stampfl, and M. J. Ford, Physical Chemistry Chemical Physics 20, (2018). [14] A. Bharathi, Y. Hariharan, J. Balaselvi, and C. Sundar, Sadhana 28, 263 (2003). [15] B. Jemima, A. Bharathi, S. Sankara, G. Reddy, Y. Hariharan, et al., in Proceedings of the DAE solid state physics symposium. V. 45 (2003). [16] S. Kazakov, R. Puzniak, K. Rogacki, A. Mironov, N. Zhigadlo, J. Jun, C. Soltmann, B. Batlogg, and J. Karpinski, Physical Review B 71, (2005). [17] S. J. Balaselvi, N. Gayathri, A. Bharathi, V. Sastry, and Y. Hariharan, Superconductor Science and Technology 17, 1401 (2004). [18] E. Ohmichi, T. Masui, S. Lee, S. Tajima, and T. Osada, Journal of the Physical Society of Japan 73, 2065 (2004). [19] A. Bharathi, S. J. Balaselvi, S. Kalavathi, G. Reddy, V. S. Sastry, Y. Hariharan, and T. Radhakrishnan, Physica C: Superconductivity 370, 211 (2002). [20] V. Braccini, A. Gurevich, J. Giencke, M. Jewell, C. Eom, D. Larbalestier, A. Pogrebnyakov, Y. Cui, B. Liu, Y. Hu, et al., Physical Review B 71, (2005). [21] M. Pissas, D. Stamopoulos, S. Lee, and S. Tajima, Physical Review B 70, (2004). [22] H. Rosner, A. Kitaigorodsky, and W. Pickett, Physical Review Letters 88, (2002). [23] A. Fogg, P. Chalker, J. Claridge, G. Darling, and M. Rosseinsky, Physical Review B 67, (2003). [24] A. M. Fogg, J. Meldrum, G. R. Darling, J. B. Claridge, and M. J. Rosseinsky, Journal of the American Chemical Society 128, (2006). [25] D. Souptel, Z. Hossain, G. Behr, W. Löser, and C. Geibel, Solid State Communications 125, 17 (2003). [26] A. Bharathi, S. J. Balaselvi, M. Premila, T. Sairam, G. Reddy, C. Sundar, and Y. Hariharan, Solid State Communications 124, 423 (2002). [27] M. Gao, Z.Y. Lu, and T. Xiang, Physical Review B 91, (2015). [28] Q.Z. Li, X.W. Yan, M. Gao, and J. Wang, Europhysics Letters 122, (2018). [29] T. Bazhirov, Y. Sakai, S. Saito, and M. L. Cohen, Physical Review B 89, (2014). [30] R. Miao, G. Huang, and J. Yang, Solid State Communications 233, 30 (2016). [31] P. Ravindran, P. Vajeeston, R. Vidya, A. Kjekshus, and H. Fjellvåg, Physical Review B 64, (2001). [32] J. P. Perdew, K. Burke, and M. Ernzerhof, Physical Review Letters 77, 3865 (1996). [33] J. P. Perdew, A. Ruzsinszky, G. I. Csonka, O. A. Vydrov, G. E. Scuseria, L. A. Constantin, X. Zhou, and K. Burke, Physical Review Letters 100, (2008). [34] P. Giannozzi, S. Baroni, N. Bonini, M. Calandra, R. Car, C. Cavazzoni, D. Ceresoli, G. L. Chiarotti, M. Cococcioni, I. Dabo, et al., Journal of Physics: Condensed Matter 21, (2009). [35] D. Vanderbilt, Physical Review B 41, 7892 (1990). [36] We use same the cutoff energy and a 666 uniform grid of qpoint for MgB 2. For calculation of the electronphonon coupling constant and Fermi surface evaluation, we use a kpoint mesh. [37] M. Kawamura, Y. Gohda, and S. Tsuneyuki, Physical Review B 89, (2014).
7 7 [38] S. Baroni, S. De Gironcoli, A. Dal Corso, and P. Giannozzi, Reviews of Modern Physics 73, 515 (2001). [39] G. Eliashberg, Sov. Phys. JETP 11, 696 (1960). [40] P. B. Allen, Physical Review B 6, 2577 (1972). [41] P. B. Allen and R. Dynes, Physical Review B 12, 905 (1975). [42] C. Richardson and N. Ashcroft, Physical Review Letters 78, 118 (1997). [43] K.H. Lee, K.J. Chang, and M. L. Cohen, Physical Review B 52, 1425 (1995). [44] The formation energy is calculated by taking the energy difference between the total energy of the compound and sum of the energy of individual constituent elements in their stable structure. We used hexagonal Mg, facecentered cubic Ca and Sr, bodycentered cubic Ba, graphite (C), and αb 12 type structure of boron [60]. Our calculated formation energies of MgBC, CaBC, SrBC and BaBC are 0.14, 0.13, 0.73 and 1.5 ev.fu 1, respectively. Although the formation energy of MgBC is small, the negative value of the formation energy of the first two compounds indicates a high possibility of synthesis of first two compounds in the laboratory. However, the positive formation energy of SrBC and BaBC indicates difficulty in the synthesis. The nonequilibrium methods of growth (epitaxial technique) may be used to synthesis these compounds (as a metastable structure), although it might be difficult. [45] I. Mazin and V. Antropov, Physica C: Superconductivity 385, 49 (2003). [46] G. Grimvall, B. MagyariKöpe, V. Ozoliņš, and K. A. Persson, Reviews of Modern Physics 84, 945 (2012). [47] N. Kato, H. Nagao, K. Nishikawa, K. Nishidate, and K. Endo, International Journal of Quantum Chemistry 96, 457 (2004). [48] The large value of electronphonon coupling of MgBC may give rise to the question of the lattice instability. All the predicted compounds have 18 independent vibrational modes. We have calculated the frequencies of each mode by using a uniform q 1 q 1 q 2 grid, where q 1 has been varied from 4 to 8 and q 2 from 2 to 4. We do not find any imaginary frequencies at these phonon wave vectors and along the considered highsymmetry kpoints. Moreover, we have calculated the phonon dispersion using a Mazari Vanderbilt smearing of width 0.08 Ry and obtained the same phonon dispersion curves. Furthermore, we have calculated the phonon dispersion using the finite displacement method in the Phonopy program [59] and obtained identical results. The obtained phonon dispersion curves suggest that XBC are dynamically stable. [49] Y. Kong, O. Dolgov, O. Jepsen, and O. Andersen, Physical Review B 64, (2001). [50] T. Yildirim, O. Gülseren, J. Lynn, C. Brown, T. Udovic, Q. Huang, N. Rogado, K. Regan, M. Hayward, J. Slusky, et al., Physical Review Letters 87, (2001). [51] A. Eiguren and C. AmbroschDraxl, Physical Review B 78, (2008). [52] M. Calandra, G. Profeta, and F. Mauri, Physical Review B 82, (2010). [53] E. R. Margine and F. Giustino, Physical Review B 87, (2013). [54] J. An and W. Pickett, Physical Review Letters 86, 4366 (2001). [55] H. J. Choi, D. Roundy, H. Sun, M. L. Cohen, and S. G. Louie, Physical Review B 66, (2002). [56] H. J. Choi, D. Roundy, H. Sun, M. L. Cohen, and S. G. Louie, Nature 418, 758 (2002). [57] K.P. Bohnen, R. Heid, and B. Renker, Physical Review Letters 86, 5771 (2001). [58] T. Morshedloo, M. Roknabadi, and M. Behdani, Physica C: Superconductivity and its Applications 509, 1 (2015). [59] A. Togo and I. Tanaka, Scripta Materialia 108, 1 (2015). [60] B. Decker and J. Kasper, Acta Crystallographica 12, 503 (1959).
Plate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationFirst Step : Identifying Pseudopotentials
Quantum Espresso Quick Start Introduction Quantum Espresso (http://www.quantumespresso.org/) is a sophisticated collection of tools for electronic structure calculations via DFT using plane waves and
More informationMatter, Materials, Crystal Structure and Bonding. Chris J. Pickard
Matter, Materials, Crystal Structure and Bonding Chris J. Pickard Why should a theorist care? Where the atoms are determines what they do Where the atoms can be determines what we can do Overview of Structure
More informationGraphene a material for the future
Graphene a material for the future by Olav Thorsen What is graphene? What is graphene? Simply put, it is a thin layer of pure carbon What is graphene? Simply put, it is a thin layer of pure carbon It has
More informationThe Application of Density Functional Theory in Materials Science
The Application of Density Functional Theory in Materials Science Slide 1 Outline Atomistic Modelling Group at MUL Density Functional Theory Numerical Details HPC Cluster at the MU Leoben Applications
More informationNo Evidence for a new phase of dense hydrogen above 325 GPa
1 No Evidence for a new phase of dense hydrogen above 325 GPa Ranga P. Dias, Ori Noked, and Isaac F. Silvera Lyman Laboratory of Physics, Harvard University, Cambridge MA, 02138 In recent years there has
More informationRelevant Reading for this Lecture... Pages 8387.
LECTURE #06 Chapter 3: Xray Diffraction and Crystal Structure Determination Learning Objectives To describe crystals in terms of the stacking of planes. How to use a dot product to solve for the angles
More informationState of the art in reactive magnetron sputtering
State of the art in reactive magnetron sputtering T. Nyberg, O. Kappertz, T. Kubart and S. Berg Solid State Electronics, The Ångström Laboratory, Uppsala University, Box 534, S751 21 Uppsala, Sweden D.
More informationAnharmonicity and Weak Mode Assignment in La 2 x Sr x CuO 4 with Oxygen Isotopic Substitution
Vol. 111 (2007) ACTA PHYSICA POLONICA A No. 1 Proceedings of the Symposium K: Complex Oxide Materials for New Technologies of EMRS Fall Meeting 2006, Warsaw, September 4 8, 2006 Anharmonicity and Weak
More informationCRYSTALLINE SOLIDS IN 3D
CRYSTALLINE SOLIDS IN 3D Andrew Baczewski PHY 491, October 7th, 2011 OVERVIEW First  are there any questions from the previous lecture? Today, we will answer the following questions: Why should we care
More informationExperiment #5: Qualitative Absorption Spectroscopy
Experiment #5: Qualitative Absorption Spectroscopy One of the most important areas in the field of analytical chemistry is that of spectroscopy. In general terms, spectroscopy deals with the interactions
More informationSEMICONDUCTOR lasers with optical feedback have
IEEE JOURNAL OF QUANTUM ELECTRONICS, VOL. 34, NO. 10, OCTOBER 1998 1979 Dynamics and Linear Stability Analysis in Semiconductor Lasers with PhaseConjugate Feedback Atsushi Murakami and Junji Ohtsubo,
More informationAccuracy of the coherent potential approximation for a onedimensional array with a Gaussian distribution of fluctuations in the onsite potential
Accuracy of the coherent potential approximation for a onedimensional array with a Gaussian distribution of fluctuations in the onsite potential I. Avgin Department of Electrical and Electronics Engineering,
More informationThe Role of Electric Polarization in Nonlinear optics
The Role of Electric Polarization in Nonlinear optics Sumith Doluweera Department of Physics University of Cincinnati Cincinnati, Ohio 45221 Abstract Nonlinear optics became a very active field of research
More informationSolid State Detectors = SemiConductor based Detectors
Solid State Detectors = SemiConductor based Detectors Materials and their properties Energy bands and electronic structure Charge transport and conductivity Boundaries: the pn junction Charge collection
More informationChapter 8 Basic Concepts of the Chemical Bonding
Chapter 8 Basic Concepts of the Chemical Bonding 1. There are paired and unpaired electrons in the Lewis symbol for a phosphorus atom. (a). 4, 2 (b). 2, 4 (c). 4, 3 (d). 2, 3 Explanation: Read the question
More informationA Beginner s Guide to Materials Studio and DFT Calculations with Castep. P. Hasnip (pjh503@york.ac.uk)
A Beginner s Guide to Materials Studio and DFT Calculations with Castep P. Hasnip (pjh503@york.ac.uk) September 18, 2007 Materials Studio collects all of its files into Projects. We ll start by creating
More informationCHAPTER 6 REVIEW. Chemical Bonding. Answer the following questions in the space provided.
Name Date lass APTER 6 REVIEW hemical Bonding SETIN 1 SRT ANSWER Answer the following questions in the space provided. 1. a A chemical bond between atoms results from the attraction between the valence
More information= N 2 = 3π2 n = k 3 F. The kinetic energy of the uniform system is given by: 4πk 2 dk h2 k 2 2m. (2π) 3 0
Chapter 1 ThomasFermi Theory The ThomasFermi theory provides a functional form for the kinetic energy of a noninteracting electron gas in some known external potential V (r) (usually due to impurities)
More informationSection 3: Crystal Binding
Physics 97 Interatomic forces Section 3: rystal Binding Solids are stable structures, and therefore there exist interactions holding atoms in a crystal together. For example a crystal of sodium chloride
More informationLecture: 33. Solidification of Weld Metal
Lecture: 33 Solidification of Weld Metal This chapter presents common solidification mechanisms observed in weld metal and different modes of solidification. Influence of welding speed and heat input on
More informationSolar Cell Parameters and Equivalent Circuit
9 Solar Cell Parameters and Equivalent Circuit 9.1 External solar cell parameters The main parameters that are used to characterise the performance of solar cells are the peak power P max, the shortcircuit
More informationInfrared Spectroscopy: Theory
u Chapter 15 Infrared Spectroscopy: Theory An important tool of the organic chemist is Infrared Spectroscopy, or IR. IR spectra are acquired on a special instrument, called an IR spectrometer. IR is used
More informationIntroduction OLEDs OTFTs OPVC Summary. Organic Electronics. Felix Buth. Walter Schottky Institut, TU München. Joint Advanced Student School 2008
Felix Buth Joint Advanced Student School 2008 Outline 1 Introduction Difference organic/inorganic semiconductors From molecular orbitals to the molecular crystal 2 Organic Light Emitting Diodes Basic Principals
More informationElements in the periodic table are indicated by SYMBOLS. To the left of the symbol we find the atomic mass (A) at the upper corner, and the atomic num
. ATOMIC STRUCTURE FUNDAMENTALS LEARNING OBJECTIVES To review the basics concepts of atomic structure that have direct relevance to the fundamental concepts of organic chemistry. This material is essential
More informationSUPERCONDUCTIVITY. PH 318 Introduction to superconductors 1
SUPERCONDUCTIVITY property of complete disappearance of electrical resistance in solids when they are cooled below a characteristic temperature. This temperature is called transition temperature or critical
More informationMechanics 1: Conservation of Energy and Momentum
Mechanics : Conservation of Energy and Momentum If a certain quantity associated with a system does not change in time. We say that it is conserved, and the system possesses a conservation law. Conservation
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationChapter Test B. Chapter: Measurements and Calculations
Assessment Chapter Test B Chapter: Measurements and Calculations PART I In the space provided, write the letter of the term or phrase that best completes each statement or best answers each question. 1.
More informationSampling the Brillouinzone:
Sampling the Brillouinzone: Andreas EICHLER Institut für Materialphysik and Center for Computational Materials Science Universität Wien, Sensengasse 8, A090 Wien, Austria binitio ienna ackage imulation
More information thus, the total number of atoms per second that absorb a photon is
Stimulated Emission of Radiation  stimulated emission is referring to the emission of radiation (a photon) from one quantum system at its transition frequency induced by the presence of other photons
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationHEAT TRANSFER ANALYSIS IN A 3D SQUARE CHANNEL LAMINAR FLOW WITH USING BAFFLES 1 Vikram Bishnoi
HEAT TRANSFER ANALYSIS IN A 3D SQUARE CHANNEL LAMINAR FLOW WITH USING BAFFLES 1 Vikram Bishnoi 2 Rajesh Dudi 1 Scholar and 2 Assistant Professor,Department of Mechanical Engineering, OITM, Hisar (Haryana)
More informationDO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS
DO PHYSICS ONLINE FROM QUANTA TO QUARKS QUANTUM (WAVE) MECHANICS Quantum Mechanics or wave mechanics is the best mathematical theory used today to describe and predict the behaviour of particles and waves.
More informationSimulation of infrared and Raman spectra
Simulation of infrared and Raman spectra, 1 Bernard Kirtman, 2 Michel Rérat, 3 Simone Salustro, 1 Marco De La Pierre, 1 Roberto Orlando, 1 Roberto Dovesi 1 1) Dipartimento di Chimica, Università di Torino
More informationFree Electron Fermi Gas (Kittel Ch. 6)
Free Electron Fermi Gas (Kittel Ch. 6) Role of Electrons in Solids Electrons are responsible for binding of crystals  they are the glue that hold the nuclei together Types of binding (see next slide)
More informationThe Fundamentals of Infrared Spectroscopy. Joe Van Gompel, PhD
TN100 The Fundamentals of Infrared Spectroscopy The Principles of Infrared Spectroscopy Joe Van Gompel, PhD Spectroscopy is the study of the interaction of electromagnetic radiation with matter. The electromagnetic
More informationDetermining the Structure of an Organic Compound
Determining the Structure of an Organic Compound The analysis of the outcome of a reaction requires that we know the full structure of the products as well as the reactants In the 19 th and early 20 th
More informationJournal of the University of Chemical Technology and Metallurgy, 42, 2, 2007. 2) are in C 1
Journal of the University of Chemical M. Georgiev, Technology D. Stoilova and Metallurgy, 42, 2, 2007, 211216 METALWATER INTERACTINS AND HYDRGEN BND STRENGTH M. Georgiev 1, D. Stoilova 2 1 University
More informationUniversity of California at Santa Cruz Electrical Engineering Department EE145L: Properties of Materials Laboratory
University of California at Santa Cruz Electrical Engineering Department EE145L: Properties of Materials Laboratory Lab 8: Optical Absorption Spring 2002 Yan Zhang and Ali Shakouri, 05/22/2002 (Based
More informationAP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts
AP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts 8.1 Types of Chemical Bonds A. Ionic Bonding 1. Electrons are transferred 2. Metals react with nonmetals 3. Ions paired have lower energy
More informationLesson 4 Measures of Central Tendency
Outline Measures of a distribution s shape modality and skewness the normal distribution Measures of central tendency mean, median, and mode Skewness and Central Tendency Lesson 4 Measures of Central
More informationStates of Matter CHAPTER 10 REVIEW SECTION 1. Name Date Class. Answer the following questions in the space provided.
CHAPTER 10 REVIEW States of Matter SECTION 1 SHORT ANSWER Answer the following questions in the space provided. 1. Identify whether the descriptions below describe an ideal gas or a real gas. ideal gas
More informationC.K. Ng. Stanford Linear Accelerator Center. and. T. Weiland. University oftechnology. FB18, Schlossgartenstr. 8. D64289, Darmstadt, Germany.
SLACPUB957005 September, 1995 Impedance of the PEPII DIP Screen C.K. Ng Stanford Linear Accelerator Center Stanford University, Stanford, CA 94309, USA and T. Weiland University oftechnology FB18,
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationAn organic semiconductor is an organic compound that possesses similar
MSE 542 Final Term Paper Title: Organic Semiconductor for Flexible Electronics Name: Chunhung Huang Introduction: An organic semiconductor is an organic compound that possesses similar properties to inorganic
More informationWe shall first regard the dense sphere packing model. 1.1. Draw a two dimensional pattern of dense packing spheres. Identify the twodimensional
Set 3: Task 1 and 2 considers many of the examples that are given in the compendium. Crystal structures derived from sphere packing models may be used to describe metals (see task 2), ionical compounds
More informationIonic Bonding Pauling s Rules and the Bond Valence Method
Ionic Bonding Pauling s Rules and the Bond Valence Method Chemistry 754 Solid State Chemistry Dr. Patrick Woodward Lecture #14 Pauling Rules for Ionic Structures Linus Pauling,, J. Amer. Chem. Soc. 51,,
More informationTheoretical investigation on armchair graphene nanoribbons. with oxygenterminated edges
Theoretical investigation on armchair graphene nanoribbons with oxygenterminated edges Hongyu Ge, Guo Wang* and Yi Liao Department of Chemistry, Capital Normal University, Beijing 100048, China * Corresponding
More information12.307. 1 Convection in water (an almostincompressible fluid)
12.307 Convection in water (an almostincompressible fluid) John Marshall, Lodovica Illari and Alan Plumb March, 2004 1 Convection in water (an almostincompressible fluid) 1.1 Buoyancy Objects that are
More informationModule 3 : Molecular Spectroscopy Lecture 13 : Rotational and Vibrational Spectroscopy
Module 3 : Molecular Spectroscopy Lecture 13 : Rotational and Vibrational Spectroscopy Objectives After studying this lecture, you will be able to Calculate the bond lengths of diatomics from the value
More informationSection 5.0 : Horn Physics. By Martin J. King, 6/29/08 Copyright 2008 by Martin J. King. All Rights Reserved.
Section 5. : Horn Physics Section 5. : Horn Physics By Martin J. King, 6/29/8 Copyright 28 by Martin J. King. All Rights Reserved. Before discussing the design of a horn loaded loudspeaker system, it is
More informationThermal unobtainiums? The perfect thermal conductor and the perfect thermal insulator
Thermal unobtainiums? The perfect thermal conductor and the perfect thermal insulator David G. Cahill Materials Research Lab and Department of Materials Science and Engineering, U. of Illinois Gratefully
More informationQuestion 4.2: Write Lewis dot symbols for atoms of the following elements: Mg, Na, B, O, N, Br.
Question 4.1: Explain the formation of a chemical bond. A chemical bond is defined as an attractive force that holds the constituents (atoms, ions etc.) together in a chemical species. Various theories
More informationEnergy Transport. Focus on heat transfer. Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids)
Energy Transport Focus on heat transfer Heat Transfer Mechanisms: Conduction Radiation Convection (mass movement of fluids) Conduction Conduction heat transfer occurs only when there is physical contact
More information12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Crystal Geometry
12.524 2003 Lec 17: Dislocation Geometry and Fabric Production 1. Bibliography: Crystal Geometry Assigned Reading: [Poirier, 1985]Chapter 2, 4. General References: [Kelly and Groves, 1970] Chapter 1. [Hirth
More informationFeature Commercial codes Inhouse codes
A simple finite element solver for thermomechanical problems Keywords: Scilab, Open source software, thermoelasticity Introduction In this paper we would like to show how it is possible to develop a
More informationSUPERCONDUCTIVITY OF VARIOUS BORIDES: THE ROLE OF STRETCHED c PARAMETER
SUPERCONDUCTIVITY OF VARIOUS BORIDES: THE ROLE OF STRETCHED c PARAMETER Monika Mudgel, V. P. S. Awana $ and H. Kishan National Physical Laboratory, Dr. K. S. Krishnan Marg, New Delhi110012, India I.
More informationExcitation transfer and energy exchange processes for modeling the FleischmannPons excess heat effect
Hagelstein, P.L. and I. Chaudhary. Excitation transfer and energy exchange processes for modeling the FleischmannPons excess heat effect. in ICCF14 International Conference on Condensed Matter Nuclear
More informationHigh Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures
High Open Circuit Voltage of MQW Amorphous Silicon Photovoltaic Structures ARGYRIOS C. VARONIDES Physics and EE Department University of Scranton 800 Linden Street, Scranton PA, 18510 United States Abstract:
More informationFUNDAMENTAL PROPERTIES OF SOLAR CELLS
FUNDAMENTAL PROPERTIES OF SOLAR CELLS January 31, 2012 The University of Toledo, Department of Physics and Astronomy SSARE, PVIC Principles and Varieties of Solar Energy (PHYS 4400) and Fundamentals of
More informationUntitled Document. 1. Which of the following best describes an atom? 4. Which statement best describes the density of an atom s nucleus?
Name: Date: 1. Which of the following best describes an atom? A. protons and electrons grouped together in a random pattern B. protons and electrons grouped together in an alternating pattern C. a core
More informationFigure 1. Diode circuit model
Semiconductor Devices Nonlinear Devices Diodes Introduction. The diode is two terminal non linear device whose IV characteristic besides exhibiting nonlinear behavior is also polarity dependent. The
More informationDURABILITY OF MORTAR LININGS IN DUCTILE IRON PIPES Durability of mortar linings
DURABILITY OF MORTAR LININGS IN DUCTILE IRON PIPES Durability of mortar linings I. S. MELAND SINTEF Civil and Environmental Engineering, Cement and Concrete, Trondheim, Norway Durability of Building Materials
More informationTypes of Epitaxy. Homoepitaxy. Heteroepitaxy
Epitaxy Epitaxial Growth Epitaxy means the growth of a single crystal film on top of a crystalline substrate. For most thin film applications (hard and soft coatings, optical coatings, protective coatings)
More informationUNIT I: INTRFERENCE & DIFFRACTION Div. B Div. D Div. F INTRFERENCE
107002: EngineeringPhysics Teaching Scheme: Lectures: 4 Hrs/week Practicals2 Hrs./week T.W.25 marks Examination Scheme: Paper50 marks (2 hrs) Online 50marks Prerequisite: Basics till 12 th Standard
More informationCHAPTER 6 Chemical Bonding
CHAPTER 6 Chemical Bonding SECTION 1 Introduction to Chemical Bonding OBJECTIVES 1. Define Chemical bond. 2. Explain why most atoms form chemical bonds. 3. Describe ionic and covalent bonding.. 4. Explain
More informationSolid State Theory Physics 545
Solid State Theory Physics 545 CRYSTAL STRUCTURES Describing periodic structures Terminology Basic Structures Symmetry Operations Ionic crystals often have a definite habit which gives rise to particular
More informationWhen the fluid velocity is zero, called the hydrostatic condition, the pressure variation is due only to the weight of the fluid.
Fluid Statics When the fluid velocity is zero, called the hydrostatic condition, the pressure variation is due only to the weight of the fluid. Consider a small wedge of fluid at rest of size Δx, Δz, Δs
More informationIntroduction to Quantum Dot Nanocrystals and Nanocrystal Solids. Nuri Yazdani, 10.03.15
Introduction to Quantum Dot Nanocrystals and Nanocrystal Solids Nuri Yazdani, 10.03.15 What is a QD Nanocrystal Time: ~15m What is a QD nanocrystal? Bulk Crystal Periodic lattice of atoms which extends
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationOrbital Dynamics coupled with JahnTeller phonons in Strongly Correlated Electron System
The 5 th Scienceweb GCOE International Symposium 1 Orbital Dynamics coupled with JahnTeller phonons in Strongly Correlated Electron System Department of Physics, Tohoku University Joji Nasu In collaboration
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationELASTIC FORCES and HOOKE S LAW
PHYS101 LAB03 ELASTIC FORCES and HOOKE S LAW 1. Objective The objective of this lab is to show that the response of a spring when an external agent changes its equilibrium length by x can be described
More informationA reinterpretation of the phase transitions in Na 2 CO 3
Acta Crystallographica Section B Structural Science ISSN 01087681 Editor: Carolyn P. Brock A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva and Gervais Chapuis Copyright International
More informationSMA5111  Compound Semiconductors Lecture 2  MetalSemiconductor Junctions  Outline Introduction
SMA5111  Compound Semiconductors Lecture 2  MetalSemiconductor Junctions  Outline Introduction Structure  What are we talking about? Behaviors: Ohmic, rectifying, neither Band picture in thermal equilibrium
More informationThe excitation in Raman spectroscopy is usually. Practical Group Theory and Raman Spectroscopy, Part II: Application of Polarization
Electronically reprinted from March 214 Molecular Spectroscopy Workbench Practical Group Theory and Raman Spectroscopy, Part II: Application of Polarization In this second installment of a twopart series
More informationMOS (metaloxidesemiconductor) 李 2003/12/19
MOS (metaloxidesemiconductor) 李 2003/12/19 Outline Structure Ideal MOS The surface depletion region Ideal MOS curves The SiO 2 Si MOS diode (real case) Structure A basic MOS consisting of three layers.
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More information1 The water molecule and hydrogen bonds in water
The Physics and Chemistry of Water 1 The water molecule and hydrogen bonds in water Stoichiometric composition H 2 O the average lifetime of a molecule is 1 ms due to proton exchange (catalysed by acids
More informationUnderstanding Poles and Zeros
MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING 2.14 Analysis and Design of Feedback Control Systems Understanding Poles and Zeros 1 System Poles and Zeros The transfer function
More informationNumerical Model for the Study of the Velocity Dependence Of the Ionisation Growth in Gas Discharge Plasma
Journal of Basrah Researches ((Sciences)) Volume 37.Number 5.A ((2011)) Available online at: www.basrascience journal.org ISSN 1817 2695 Numerical Model for the Study of the Velocity Dependence Of the
More information2. Spin Chemistry and the Vector Model
2. Spin Chemistry and the Vector Model The story of magnetic resonance spectroscopy and intersystem crossing is essentially a choreography of the twisting motion which causes reorientation or rephasing
More informationCapacitance and Ferroelectrics
Ram Seshadri MRL 2031, x6129 seshadri@mrl.ucsb.edu; http://www.mrl.ucsb.edu/ seshadri/teach.html Capacitance and Ferroelectrics A voltage V applied across a capacitor of caacitance C allows a quantity
More informationTR1030. Technical Report. Thermodynamic properties of copper compounds with oxygen and hydrogen from first principles
Technical Report TR1030 Thermodynamic properties of copper compounds with oxygen and hydrogen from first principles P A Korzhavyi, B Johansson Applied Materials Physics Department of Materials Science
More informationLesson 3: Isothermal Hydrostatic Spheres. B68: a selfgravitating stable cloud. Hydrostatic selfgravitating spheres. P = "kt 2.
Lesson 3: Isothermal Hydrostatic Spheres B68: a selfgravitating stable cloud Bok Globule Relatively isolated, hence not many external disturbances Though not main mode of star formation, their isolation
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationThe Raman Fingerprint of Graphene
The Raman Fingerprint of Graphene A. C. Ferrari 1, J. C. Meyer 2, V. Scardaci 1, C. Casiraghi 1, M. Lazzeri 3, F. Mauri 3, S. Piscanec 1, D. Jiang 4, K. S. Novoselov 4, S. Roth 2, A. K. Geim 4 1 Department
More informationCopyright 2011 Casa Software Ltd. www.casaxps.com. Centre of Mass
Centre of Mass A central theme in mathematical modelling is that of reducing complex problems to simpler, and hopefully, equivalent problems for which mathematical analysis is possible. The concept of
More informationChapter 17: Light and Image Formation
Chapter 17: Light and Image Formation 1. When light enters a medium with a higher index of refraction it is A. absorbed. B. bent away from the normal. C. bent towards from the normal. D. continues in the
More informationThe quantum mechanics of particles in a periodic potential: Bloch s theorem
Handout 2 The quantum mechanics of particles in a periodic potential: Bloch s theorem 2.1 Introduction and health warning We are going to set up the formalism for dealing with a periodic potential; this
More informationComputer lab: Density functional perturbation theory. theory for lattice dynamics
Computer lab: density functional perturbation theory for lattice dynamics SISSA and DEMOCRITOS Trieste (Italy) Outline 1 The dynamical matrix 2 3 4 5 Dynamical matrix We want to write a small computer
More informationNumerical Analysis of the Moving Formwork Bracket Stress during Construction of a Curved Continuous Box Girder Bridge with Variable Width
Modern Applied Science; Vol. 9, No. 6; 2015 ISSN 19131844 EISSN 19131852 Published by Canadian Center of Science and Education Numerical Analysis of the Moving Formwork Bracket Stress during Construction
More informationLecture 3: Optical Properties of Bulk and Nano. 5 nm
Lecture 3: Optical Properties of Bulk and Nano 5 nm The Previous Lecture Origin frequency dependence of χ in real materials Lorentz model (harmonic oscillator model) 0 e  n( ) n' n '' n ' = 1 + Nucleus
More informationarxiv:1207.6196v1 [condmat.suprcon] 26 Jul 2012
Electron and phonon bandstructure calculations for the antipolar t 3 antiperovskite superconductor: Evidence of lowenergy twodimensional phonons ChangJong Kang 1, KyoHoon Ahn, KwanWoo Lee,3, B. I.
More informationLecture 3: Optical Properties of Bulk and Nano. 5 nm
Lecture 3: Optical Properties of Bulk and Nano 5 nm First H/W#1 is due Sept. 10 Course Info The Previous Lecture Origin frequency dependence of χ in real materials Lorentz model (harmonic oscillator model)
More informationPUMPED Nd:YAG LASER. Last Revision: August 21, 2007
PUMPED Nd:YAG LASER Last Revision: August 21, 2007 QUESTION TO BE INVESTIGATED: How can an efficient atomic transition laser be constructed and characterized? INTRODUCTION: This lab exercise will allow
More informationNanopore structure characterization of shales using gas adsorption and mercury intrusion techniques
Available online www.jocpr.com Journal of Chemical and Pharmaceutical Research, 2014, 6(4):850857 Research Article ISSN : 09757384 CODEN(USA) : JCPRC5 Nanopore structure characterization of shales using
More informationChapter 5. Second Edition ( 2001 McGrawHill) 5.6 Doped GaAs. Solution
Chapter 5 5.6 Doped GaAs Consider the GaAs crystal at 300 K. a. Calculate the intrinsic conductivity and resistivity. Second Edition ( 2001 McGrawHill) b. In a sample containing only 10 15 cm 3 ionized
More information